# copolymer composition - caltechauthors ... copolymer composition and sequence then reduces to the...

Post on 04-Apr-2020

0 views

Embed Size (px)

TRANSCRIPT

COPOLYMER COMPOSITION

A Chapter in

Comprehensive Polymer Science

by

David A. Tirrell Department of Polymer Science and Engineering

University of Massachusetts Anherst, MA 01003 USA

1

The successful synthesis of new materials via free radical copolymerization requires a

thorough understanding of the factors that control the structures of copolymer chains. Of the

primary structural variables used to describe polymer chains, two (copolymer composition and

comonomer sequence distribution) are unique to copolymers. The present chapter examines the

compositions and sequences of copolymers prepared via free-radical processes.

The products of free radical copolymerizations are, with few exceptions, determined by the

kinetics, rather than the thermodynamics, of the chain growth process. The problem of predicting

copolymer composition and sequence then reduces to the writing of a set of differential equations

that describe the rates at which each of the two monomers enters the copolymer chain by attack of

the growing macroradical. This requires a kinetic model of the copolymerization process, and

several such models have been described in the copolymerization literature. The following sections

examine the fundamental bases of the most important of these models, and assess the degree to

which such models can account for experimentally observed copolymerization behavior.

TERMINAL MODEL

Theory. The standard kinetic treatment of free radical copolymerization was introduced in

1944, in papers contibuted independently by Mayo and Lewis) by Alfrey and Goldfinger2 and by

~ a l 1 . 3 Following earlier suggestions by ~ostal," by Norrish and ~rookman,S and by ~enckel?

Mayo and Lewis described their experimental work on the radical copolymerization of styrene and

methyl methacrylate in terms of a model in which the rate constant for addition of each monomer

was assumed to be dependent on the identity of the terminal unit on the growing chain. Four

elementary propagation steps were then considered (Eqns 1 -4):

2

By writing differential equations that describe the rates of disappearance of monomers M1 and M2,

and by assuming steady-state concentrations of the radical centers MI* and My, one arrives at a

simple expression that relates the ratio of monomers in the copolymer (d[Ml]/d.[M2]) to the

concentrations of monomers in the feed mixture ([MI] and [Mz]) (Eqn 5):

d.[M11 [Mil r1[M11 + [M21 - - - - d[M21 [M21 [Mil + r2[M21

The parameters rl and 1-2 are reactivity ratios defined as:

ri = kiik12 and r2 = k22k21 (6)

A detailed derivation of Eqn 5 is given in Ch. 2 of this volume. (EDITOR: This is intended to

refer the reader to Prof. Harnielec's chapter.)

Analysis of the terminal model is readily extended to the prediction of copolymer sequence

distribution. Sequence distributions are most generally and conveniently specified in terms of the

number fractions of uninterrupted sequences of a given monomer (M.1 or M2) that are of a

particular length. The number fraction is of course identical to the probability that a given

uninterrupted sequence, selected at random, is of that length. Consider a sequence of M1 units of

length x. Such a sequence arises in the terminal model when a growing macroradical terminating

in Mi* adds (x - 1) Mi's followed by an M2. The probability that such a sequence forms is

obtained as the product of the probabilities of each of the independent steps that lead to the

sequence. Thus the number fraction of sequences of Mi of length x (Nxl) is given as:

~ , 1 = ~ ~ ~ ( x - 1 ) ~ ~ ~ (7)

where Pi1 is the probability that -Mi* adds Mi:

and P12 (= 1 - Pi 1) is the probability that -MI* adds M2. The lengths of M2 sequences are

determined in similar fashion, such that:

Thus Eqns 8 and 9 allow calculation of the comonomer sequence distribution from a knowledge of

the terminal model reactivity ratios and the monomer feed composition. Use of Eqns 5, 8 and 9 is

of course restricted to conditions under which the monomer feed composition is fixed. In practical

terms, this requires the use of low monomer conversions in order to avoid serious errors arising

from compositional drift as Mi and M2 enter the copolymer chain at different rates. Use of the

integrated form of Eqn 5 has been recommended in order to relax the low-conversion restriction

(cf. Ch. 2 of this volume) (EDITOR: Refer to Hamielec chapter.)

Experiment. The terminal model has proven remarkably successful in correlating a large

body of copolymerization data. Greenley7 has provided the most recent tabulation of free-radical

reactivity ratios, in which some 900 ratios were recalculated, via the equations of Kelen and

~udos,89 from the original experimental data. Table I lists some representative reactivity ratios for

several of the most important vinyl monomers.

TABLE I HERE

The data in Table I provide several important insights regarding the current status of our

understanding of radical copolymerization. First, the observed reactivity patterns may be divided

into a rather small number of classes, which may be distinguished from one another on the basis of

the magnitudes of rl and 1-2. The most useful classification is as follows.

r l = r2 = 1 (kll = kl2; k21 = k22): Neither radical center shows substantial preference

for either M1 or M2, so that the relative rates of monomer consumption are determined only by the

relative monomer concentrations in the feed mixture. Eqn 5 simplifies to:

and the copolymer and monomer feed compositions are thus identical. Of the copolymerization

systems listed in Table I, butadiene-styrene (rl = 1.35- 1.83; 1-2 = 0.37-0.84) and vinyl acetate-

vinyl chloride (rl = 0.24-0.98; r2 = 1.03-2.30) approach this pattern most closely. Each shows

4

small but signficant deviations, however, so that compositional drift with conversion becomes an

important practical concern.

r l = r2= 0 (kl l = k22 = 0): Each of the radical centers shows a strong preference for

cross-propagation. In the extreme case, the copolymer is perfectly alternating and of 1: 1

composition, regardless of the composition of the monomer feed mixture. Eqn 5 simplifies to:

The copolymerization of maleic anhydride (rl = 0.00-0.02) with styrene (r2 = 0.00-0.097) behaves

in this manner.

r l > 1; r2 < 1 (k l l > k12; k21 > k22): Each of the radical centers prefers to add Mi,

so that the copolymer is always enriched in M1 relative to the feed. This situation arises frequently

in radical copolymerization, and many examples may be found in Table I. A special case is that in

which rlr2 = 1 (kll/kl2 = k21/k22); i.e., in which both active centers show the same preference for

addition of one of the monomers. Eqn 5 then becomes:

This behavior is often termed ideal copolymerization.

r l c 1; 1-2 c 1 (k12 > kl l , k21 > k22): Each of the radical centers prefers cross-

propagation, but the preference is not absolute. This results in a tendency toward alternation,

which grows stronger as rl and r2 approach zero. The copolymerization of acryloniaile (rl =

0.00-0.17) with styrene (1-2 = 0.29-0.55) provides a good example. A characteristic of such

copolymerizations is the existence of the so-called azeotropic composition, at which the copolymer

and feed compositions are equal. This situation arises when:

which requires that:

so that:

at the azeotropic point. The azeotropic composition is of some practical significance in that at this

point compositional drift with conversion may be neglected. This allows batch copolymerizations

to be run to high conversions without the introduction of substantial compositional heterogeneity

into the product (cf. Ch. 2; EDITOR: Refer to Hamielec).

The patterns of copolymerization behavior discussed above are summarized most succinctly

in the form of composition curves in which copolymer composition (e.g., as mole fraction M1 in

the copolymer) is plotted as a function of the monomer feed composition (as mole fraction M1 in

the feed). Figure 1 shows schematic composition curves for each of the four classes of

copolymerizations described above. Such composition curves, calculated via Eqn 5, reproduce in

satisfactory fashion the experimental compositions obtained in the vast majority of radical

copolymerizations. Thus the terminal model is extraordinarily useful as a context in which to

describe the compositions of copolymers prepared from vinyl monomers of widely varying

structure and reactivity. On the other hand, the model is not as successful in the prediction of

comonomer sequence distribution1 l4 and overall copolymerization rate.115

A second point that becomes apparent on examination of Table I is that the experimentally

reported reactivity ratios, even for these most common vinyl monomers, span some range. It is

not at all uncommon for the highest and lowest reported values to differ by a factor of 2 for a given

copolymerization, a

Recommended